LMucko/crystallography-open-database huggingface dataset:
The particularities of infinite-layer compounds Sr1-x Lnx Cu O2-d (Ln = La, Pr, Nd, Eu)
Luparev, V.V.; Kuz'micheva, G.M.; Khlybov, E.P.; Kostyleva, I.E.; Palewski, T.; Crystal Research and Technology 36 (2001) 557–564; doi:

data_1525871
_publ_section_title
;
 The particularities of infinite-layer compounds Sr1-x Lnx Cu O2-d (Ln =
 La, Pr, Nd, Eu)
;
_journal_name_full               'Crystal Research and Technology'
_journal_page_first              557
_journal_page_last               564
_journal_volume                  36
_journal_year                    2001
_chemical_formula_sum            'Cu Eu0.02 O1.96 Sr0.98'
_chemical_name_systematic        '(Sr0.98 Eu0.02) Cu O1.96'
_space_group_IT_number           123
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.93
_cell_length_b                   3.93
_cell_length_c                   3.426
_cell_volume                     52.914
_citation_journal_id_ASTM        CRTEDF
_cod_data_source_file            Luparev_CRTEDF_2001_978.cif
_cod_data_source_block           Cu1Eu0.02O1.96Sr0.98
_cod_original_cell_volume        52.91423
_cod_original_formula_sum        'Cu1 Eu0.02 O1.96 Sr0.98'
_cod_database_code               1525871
An effective harmonic potential for aluminophosphate molecular sieves : application to Al P O4-5
Demontis, P.; Gulin Gonzalez, J.; de las Pozas, C.; Tilocca, A.; Suffritti, G.B.; Microporous and Mesoporous Materials 42 (2001) 103–111; doi:

data_1525872
_publ_section_title
;
 An effective harmonic potential for aluminophosphate molecular sieves :
 application to Al P O4-5
;
_journal_name_full               'Microporous and Mesoporous Materials'
_journal_page_first              103
_journal_page_last               111
_journal_volume                  42
_journal_year                    2001
_chemical_formula_sum            'Al O4 P'
_chemical_name_systematic        'Al (P O4)'
_space_group_IT_number           27
_symmetry_space_group_name_Hall  'P 2 -2c'
_symmetry_space_group_name_H-M   'P c c 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            24
_cell_length_a                   13.794
_cell_length_b                   23.9
_cell_length_c                   8.417
_cell_volume                     2774.888
_citation_journal_id_ASTM        MIMMFJ
_cod_data_source_file            Demontis_MIMMFJ_2001_1768.cif
_cod_data_source_block           Al1O4P1
_cod_original_formula_sum        'Al1 O4 P1'
_cod_database_code               1525872
The particularities of infinite-layer compounds Sr1-x Lnx Cu O2-d (Ln = La, Pr, Nd, Eu)
Luparev, V.V.; Khlybov, E.P.; Kuz'micheva, G.M.; Palewski, T.; Kostyleva, I.E.; Crystal Research and Technology 36 (2001) 557–564; doi:

data_1525873
_publ_section_title
;
 The particularities of infinite-layer compounds Sr1-x Lnx Cu O2-d (Ln =
 La, Pr, Nd, Eu)
;
_journal_name_full               'Crystal Research and Technology'
_journal_page_first              557
_journal_page_last               564
_journal_volume                  36
_journal_year                    2001
_chemical_formula_sum            'Cu Eu0.21 O1.94 Sr0.79'
_chemical_name_systematic        '(Sr0.79 Eu0.21) Cu O1.94'
_space_group_IT_number           123
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.9421
_cell_length_b                   3.9421
_cell_length_c                   3.371
_cell_volume                     52.386
_citation_journal_id_ASTM        CRTEDF
_cod_data_source_file            Luparev_CRTEDF_2001_979.cif
_cod_data_source_block           Cu1Eu0.21O1.94Sr0.79
_cod_original_cell_volume        52.38586
_cod_original_formula_sum        'Cu1 Eu0.21 O1.94 Sr0.79'
_cod_database_code               1525873
Rare earth fluorosulfides Ln S F and Ln2 A F4 S2 as new colour pigments
Demourgues, A.; Tressaud, A.; Laronze, H.; Macaudiere, P.; Journal of Alloys Compd. 323 (2001) 223–230; doi:

data_1525874
_publ_section_title
;
 Rare earth fluorosulfides Ln S F and Ln2 A F4 S2 as new colour pigments
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              223
_journal_page_last               230
_journal_volume                  323
_journal_year                    2001
_chemical_formula_sum            'F La S'
_chemical_name_systematic        'La S F'
_space_group_IT_number           129
_symmetry_space_group_name_Hall  '-P 4a 2a'
_symmetry_space_group_name_H-M   'P 4/n m m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.0398
_cell_length_b                   4.0398
_cell_length_c                   6.9697
_cell_volume                     113.745
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Demourgues_JALCEU_2001_1301.cif
_cod_data_source_block           F1La1S1
_cod_original_cell_volume        113.7454
_cod_original_formula_sum        'F1 La1 S1'
_cod_database_code               1525874
Crystal structure of (Hg, Ce, Cu) (Sr, Pr)2 (Pr, Sr) Cu2 O6+d and (Hg, vac) (Sr, Pr)2 (Pr, Sr)2 Cu3 O8+d phases
Luparev, V.V.; Kuz'micheva, G.M.; Zhurnal Strukturnoi Khimii (Issue-No. from 1981) 41 (2000) 1219–1232; doi:

data_1525875
_publ_section_title
;
 Crystal structure of (Hg, Ce, Cu) (Sr, Pr)2 (Pr, Sr) Cu2 O6+d and (Hg,
 vac) (Sr, Pr)2 (Pr, Sr)2 Cu3 O8+d phases
;
_journal_name_full
'Zhurnal Strukturnoi Khimii (Issue-No. from 1981)'
_journal_page_first              1219
_journal_page_last               1232
_journal_volume                  41
_journal_year                    2000
_chemical_formula_sum            'Ce0.31 Cu2.25 Hg0.44 O7 Pr0.72 Sr2.28'
_chemical_name_systematic
;
(Hg0.44 Ce0.31 Cu0.25) (Sr0.9 Pr0.1)2 (Pr0.52 Sr0.48) Cu2 O7
;
_space_group_IT_number           123
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.8634
_cell_length_b                   3.8634
_cell_length_c                   12.203
_cell_volume                     182.140
_citation_journal_id_ASTM        ZSTKAI
_cod_data_source_file            Luparev_ZSTKAI_2000_862.cif
_cod_data_source_block           Ce0.31Cu2.25Hg0.44O7Pr0.72Sr2.28
_cod_original_cell_volume        182.1403
_cod_database_code               1525875
Rare earth fluorosulfides Ln S F and Ln2 A F4 S2 as new colour pigments
Demourgues, A.; Tressaud, A.; Laronze, H.; Macaudiere, P.; Journal of Alloys Compd. 323 (2001) 223–230; doi:

data_1525876
_publ_section_title
;
 Rare earth fluorosulfides Ln S F and Ln2 A F4 S2 as new colour pigments
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              223
_journal_page_last               230
_journal_volume                  323
_journal_year                    2001
_chemical_formula_sum            'F Pr S'
_chemical_name_systematic        'Pr S F'
_space_group_IT_number           129
_symmetry_space_group_name_Hall  '-P 4a 2a'
_symmetry_space_group_name_H-M   'P 4/n m m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   3.9569
_cell_length_b                   3.9569
_cell_length_c                   6.9226
_cell_volume                     108.388
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Demourgues_JALCEU_2001_1302.cif
_cod_data_source_block           F1Pr1S1
_cod_original_cell_volume        108.3875
_cod_original_formula_sum        'F1 Pr1 S1'
_cod_database_code               1525876
Crystal structure of (Hg, Ce, Cu) (Sr, Pr)2 (Pr, Sr) Cu2 O6+d and (Hg, vac) (Sr, Pr)2 (Pr, Sr)2 Cu3 O8+d phases
Luparev, V.V.; Kuz'micheva, G.M.; Zhurnal Strukturnoi Khimii (Issue-No. from 1981) 41 (2000) 1219–1232; doi:

data_1525877
_publ_section_title
;
 Crystal structure of (Hg, Ce, Cu) (Sr, Pr)2 (Pr, Sr) Cu2 O6+d and (Hg,
 vac) (Sr, Pr)2 (Pr, Sr)2 Cu3 O8+d phases
;
_journal_name_full
'Zhurnal Strukturnoi Khimii (Issue-No. from 1981)'
_journal_page_first              1219
_journal_page_last               1232
_journal_volume                  41
_journal_year                    2000
_chemical_formula_sum            'Cu3 Hg0.36 O9.36 Pr2.26 Sr1.74'
_chemical_name_systematic
'Hg0.36 (Sr0.5 Pr0.5)2 (Pr0.63 Sr0.37)2 Cu3 O9.36'
_space_group_IT_number           123
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.8464
_cell_length_b                   3.8464
_cell_length_c                   15.2615
_cell_volume                     225.791
_citation_journal_id_ASTM        ZSTKAI
_cod_data_source_file            Luparev_ZSTKAI_2000_863.cif
_cod_data_source_block           Cu3Hg0.36O9.36Pr2.26Sr1.74
_cod_original_cell_volume        225.7907
_cod_database_code               1525877
Rare earth fluorosulfides Ln S F and Ln2 A F4 S2 as new colour pigments
Demourgues, A.; Tressaud, A.; Laronze, H.; Macaudiere, P.; Journal of Alloys Compd. 323 (2001) 223–230; doi:

data_1525878
_publ_section_title
;
 Rare earth fluorosulfides Ln S F and Ln2 A F4 S2 as new colour pigments
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              223
_journal_page_last               230
_journal_volume                  323
_journal_year                    2001
_chemical_formula_sum            'F Nd S'
_chemical_name_systematic        'Nd S F'
_space_group_IT_number           129
_symmetry_space_group_name_Hall  '-P 4a 2a'
_symmetry_space_group_name_H-M   'P 4/n m m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   3.9278
_cell_length_b                   3.9278
_cell_length_c                   6.9056
_cell_volume                     106.537
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Demourgues_JALCEU_2001_1303.cif
_cod_data_source_block           F1Nd1S1
_cod_original_cell_volume        106.5369
_cod_original_formula_sum        'F1 Nd1 S1'
_cod_database_code               1525878
Crystal structure of (Hg, Ce, Cu) (Sr, Pr)2 (Pr, Sr) Cu2 O6+d and (Hg, vac) (Sr, Pr)2 (Pr, Sr)2 Cu3 O8+d phases
Luparev, V.V.; Kuz'micheva, G.M.; Zhurnal Strukturnoi Khimii (Issue-No. from 1981) 41 (2000) 1219–1232; doi:

data_1525879
_publ_section_title
;
 Crystal structure of (Hg, Ce, Cu) (Sr, Pr)2 (Pr, Sr) Cu2 O6+d and (Hg,
 vac) (Sr, Pr)2 (Pr, Sr)2 Cu3 O8+d phases
;
_journal_name_full
'Zhurnal Strukturnoi Khimii (Issue-No. from 1981)'
_journal_page_first              1219
_journal_page_last               1232
_journal_volume                  41
_journal_year                    2000
_chemical_formula_sum            'Cu3 Hg0.29 O9.32 Pr1.88 Sr2.12'
_chemical_name_systematic
'Hg0.29 (Sr0.67 Pr0.33)2 (Pr0.61 Sr0.39)2 Cu3 O9.32'
_space_group_IT_number           47
_symmetry_space_group_name_Hall  '-P 2 2'
_symmetry_space_group_name_H-M   'P m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.8294
_cell_length_b                   3.8567
_cell_length_c                   15.2763
_cell_volume                     225.613
_citation_journal_id_ASTM        ZSTKAI
_cod_data_source_file            Luparev_ZSTKAI_2000_864.cif
_cod_data_source_block           Cu3Hg0.29O9.32Pr1.88Sr2.12
_cod_original_cell_volume        225.6133
_cod_database_code               1525879
Rare earth fluorosulfides Ln S F and Ln2 A F4 S2 as new colour pigments
Demourgues, A.; Tressaud, A.; Laronze, H.; Macaudiere, P.; Journal of Alloys Compd. 323 (2001) 223–230; doi:

data_1525880
_publ_section_title
;
 Rare earth fluorosulfides Ln S F and Ln2 A F4 S2 as new colour pigments
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              223
_journal_page_last               230
_journal_volume                  323
_journal_year                    2001
_chemical_formula_sum            'F Gd S'
_chemical_name_systematic        'Gd S F'
_space_group_IT_number           129
_symmetry_space_group_name_Hall  '-P 4a 2a'
_symmetry_space_group_name_H-M   'P 4/n m m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   3.8297
_cell_length_b                   3.8297
_cell_length_c                   6.8529
_cell_volume                     100.509
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Demourgues_JALCEU_2001_1304.cif
_cod_data_source_block           F1Gd1S1
_cod_original_cell_volume        100.5088
_cod_original_formula_sum        'F1 Gd1 S1'
_cod_database_code               1525880
Crystal structure of (Hg, Ce, Cu) (Sr, Pr)2 (Pr, Sr) Cu2 O6+d and (Hg, vac) (Sr, Pr)2 (Pr, Sr)2 Cu3 O8+d phases
Luparev, V.V.; Kuz'micheva, G.M.; Zhurnal Strukturnoi Khimii (Issue-No. from 1981) 41 (2000) 1219–1232; doi:

data_1525881
_publ_section_title
;
 Crystal structure of (Hg, Ce, Cu) (Sr, Pr)2 (Pr, Sr) Cu2 O6+d and (Hg,
 vac) (Sr, Pr)2 (Pr, Sr)2 Cu3 O8+d phases
;
_journal_name_full
'Zhurnal Strukturnoi Khimii (Issue-No. from 1981)'
_journal_page_first              1219
_journal_page_last               1232
_journal_volume                  41
_journal_year                    2000
_chemical_formula_sum            'Cu3 Hg0.29 O9 Pr1.8 Sr2.2'
_chemical_name_systematic
'Hg0.29 (Sr0.61 Pr0.39)2 (Pr0.51 Sr0.49)2 Cu3 O9'
_space_group_IT_number           47
_symmetry_space_group_name_Hall  '-P 2 2'
_symmetry_space_group_name_H-M   'P m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.8294
_cell_length_b                   3.8567
_cell_length_c                   15.2763
_cell_volume                     225.613
_citation_journal_id_ASTM        ZSTKAI
_cod_data_source_file            Luparev_ZSTKAI_2000_865.cif
_cod_data_source_block           Cu3Hg0.29O9Pr1.8Sr2.2
_cod_original_cell_volume        225.6133
_cod_database_code               1525881
Rare earth fluorosulfides Ln S F and Ln2 A F4 S2 as new colour pigments
Demourgues, A.; Tressaud, A.; Laronze, H.; Macaudiere, P.; Journal of Alloys Compd. 323 (2001) 223–230; doi:

data_1525882
_publ_section_title
;
 Rare earth fluorosulfides Ln S F and Ln2 A F4 S2 as new colour pigments
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              223
_journal_page_last               230
_journal_volume                  323
_journal_year                    2001
_chemical_formula_sum            'Ce2 F4 S2 Sr'
_chemical_name_systematic        'Ce2 Sr F4 S2'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.0782
_cell_length_b                   4.0782
_cell_length_c                   19.637
_cell_volume                     326.597
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Demourgues_JALCEU_2001_1305.cif
_cod_data_source_block           Ce2F4S2Sr1
_cod_original_formula_sum        'Ce2 F4 S2 Sr1'
_cod_database_code               1525882
Structure refinement of astrophyllite
Ma, Z.-S.; Li, G.-W.; Zhou, H.-Y.; Shi, N.-C.; Pushcharovskii, D.Yu.; Ye, D.-I.; Science in China Series D 44 (2001) 508–516; doi:

data_1525883
_publ_section_title
;
 Structure refinement of astrophyllite
;
_journal_name_full               'Science in China Series D'
_journal_page_first              508
_journal_page_last               516
_journal_volume                  44
_journal_year                    2001
_chemical_formula_sum            'Fe6.314 H4 K1.875 Na O31 Si8 Ti2'
_chemical_name_systematic        'Fe6.314 K1.875 Na (Ti2 Si8 O24) (O3 (O H)4)'
_space_group_IT_number           1
_symmetry_space_group_name_Hall  'P 1'
_symmetry_space_group_name_H-M   'P 1'
_cell_angle_alpha                113.16
_cell_angle_beta                 103.04
_cell_angle_gamma                94.56
_cell_formula_units_Z            1
_cell_length_a                   5.359
_cell_length_b                   11.614
_cell_length_c                   11.861
_cell_volume                     649.457
_citation_journal_id_ASTM        SCDEF8
_cod_data_source_file            Ma_SCDEF8_2001_1940.cif
_cod_data_source_block           H4Fe6.314K1.875Na1O31Si8Ti2
_cod_original_cell_volume        649.4567
_cod_original_formula_sum        'H4 Fe6.314 K1.875 Na1 O31 Si8 Ti2'
_cod_database_code               1525883
Preparation and structural properties of new series of mixed-anion compounds : rare earth fluorosulfides
Demourgues, A.; Tressaud, A.; Laronze, H.; Gravereau, P.; Macaudiere, P.; Journal of Fluorine Chemistry 107 (2001) 215–221; doi:

data_1525884
_publ_section_title
;
 Preparation and structural properties of new series of mixed-anion
 compounds : rare earth fluorosulfides
;
_journal_name_full               'Journal of Fluorine Chemistry'
_journal_page_first              215
_journal_page_last               221
_journal_volume                  107
_journal_year                    2001
_chemical_formula_sum            'Ce F S'
_chemical_name_systematic        'Ce S F'
_space_group_IT_number           129
_symmetry_space_group_name_Hall  '-P 4a 2a'
_symmetry_space_group_name_H-M   'P 4/n m m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   3.9917
_cell_length_b                   3.9917
_cell_length_c                   6.9473
_cell_volume                     110.696
_citation_journal_id_ASTM        JFLCAR
_cod_data_source_file            Demourgues_JFLCAR_2001_1381.cif
_cod_data_source_block           Ce1F1S1
_cod_original_formula_sum        'Ce1 F1 S1'
_cod_database_code               1525884
Neutron investigation of Tb1-x Cax Mn O3 (x >= 0.5)
Machida, A.; Moritomo, Y.; Ohoyama, K.; Nakamura, A.; Journal of the Physical Society of Japan 70 (2001) 3739–3746; doi:

data_1525885
_publ_section_title
;
 Neutron investigation of Tb1-x Cax Mn O3 (x >= 0.5)
;
_journal_name_full               'Journal of the Physical Society of Japan'
_journal_page_first              3739
_journal_page_last               3746
_journal_volume                  70
_journal_year                    2001
_chemical_formula_sum            'Ca0.5 Mn O2.991 Tb0.5'
_chemical_name_systematic        '(Tb0.5 Ca0.5) Mn O2.991'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.3338
_cell_length_b                   5.4584
_cell_length_c                   7.4666
_cell_volume                     217.383
_citation_journal_id_ASTM        JUPSAU
_cod_data_source_file            Machida_JUPSAU_2001_1822.cif
_cod_data_source_block           Ca0.5Mn1O2.991Tb0.5
_cod_original_cell_volume        217.3827
_cod_original_sg_symbol_Hall     '-P 2ac 2n (z,x,y)'
_cod_original_formula_sum        'Ca0.5 Mn1 O2.991 Tb0.5'
_cod_database_code               1525885
Preparation and structural properties of new series of mixed-anion compounds : rare earth fluorosulfides
Demourgues, A.; Laronze, H.; Tressaud, A.; Gravereau, P.; Macaudiere, P.; Journal of Fluorine Chemistry 107 (2001) 215–221; doi:

data_1525886
_publ_section_title
;
 Preparation and structural properties of new series of mixed-anion
 compounds : rare earth fluorosulfides
;
_journal_name_full               'Journal of Fluorine Chemistry'
_journal_page_first              215
_journal_page_last               221
_journal_volume                  107
_journal_year                    2001
_chemical_formula_sum            'F S Sm'
_chemical_name_systematic        'Sm S F'
_space_group_IT_number           129
_symmetry_space_group_name_Hall  '-P 4a 2a'
_symmetry_space_group_name_H-M   'P 4/n m m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   3.8723
_cell_length_b                   3.8723
_cell_length_c                   6.8755
_cell_volume                     103.096
_citation_journal_id_ASTM        JFLCAR
_cod_data_source_file            Demourgues_JFLCAR_2001_1382.cif
_cod_data_source_block           F1S1Sm1
_cod_original_cell_volume        103.0961
_cod_original_formula_sum        'F1 S1 Sm1'
_cod_database_code               1525886
Neutron investigation of Tb1-x Cax Mn O3 (x >= 0.5)
Machida, A.; Moritomo, Y.; Ohoyama, K.; Nakamura, A.; Journal of the Physical Society of Japan 70 (2001) 3739–3746; doi:

data_1525887
_publ_section_title
;
 Neutron investigation of Tb1-x Cax Mn O3 (x >= 0.5)
;
_journal_name_full               'Journal of the Physical Society of Japan'
_journal_page_first              3739
_journal_page_last               3746
_journal_volume                  70
_journal_year                    2001
_chemical_formula_sum            'Ca0.55 Mn O2.973 Tb0.45'
_chemical_name_systematic        '(Tb0.45 Ca0.55) Mn O2.973'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.3255
_cell_length_b                   5.4277
_cell_length_c                   7.4653
_cell_volume                     215.786
_citation_journal_id_ASTM        JUPSAU
_cod_data_source_file            Machida_JUPSAU_2001_1823.cif
_cod_data_source_block           Ca0.55Mn1O2.973Tb0.45
_cod_original_cell_volume        215.7861
_cod_original_sg_symbol_Hall     '-P 2ac 2n (z,x,y)'
_cod_original_formula_sum        'Ca0.55 Mn1 O2.973 Tb0.45'
_cod_database_code               1525887